Developing constitutive model parameters via a multi-scale approach
- B. S. Anglin^{1}Email author,
- B. T. Gockel^{2, 3} and
- A. D. Rollett^{3}
DOI: 10.1186/s40192-016-0053-4
© The Author(s). 2016
Received: 7 April 2016
Accepted: 18 May 2016
Published: 19 July 2016
Abstract
Computing the mechanical response of materials requires accurate constitutive descriptions, especially their plastic behavior. Furthermore, the ability of a model to be used as a predictive, rather than a descriptive, tool motivates the development of physically based constitutive models. This work investigates combining a homogenized viscoplastic self-consistent (VPSC) approach to reduce the development time for a high-resolution viscoplastic model based on the fast Fourier transform (FFT). An optimization scheme based on a least-squares algorithm is presented. The constitutive responses of copper, interstitial-free steel, and pearlite are investigated, and the model parameters are presented. Optimized parameters from the low-fidelity model provide close agreement (<2 MPa, ~1 % error) with stress-strain data at low strains (<10 %) in the high-fidelity FFT model. Simple adjustments to constitutive law parameters bring the FFT stress-strain curve in alignment with experimental data at strains greater than 10 %. A two-phase constitutive law is developed for a pearlitic steel using a single stress-strain curve, supplemented by data for the constituent phases. Sources of error and methods of using material information are discussed that lead to optimal estimates of initial parameter values.
Keywords
Optimization Constitutive law Pearlite Viscoplastic Multi-scaleBackground
The usefulness and predictive value of a material model is dependent on two factors: the range over which the description of the mechanisms and physics included in the model are applicable and the parameters used to accurately tune a model to measured results. The determination of the latter has been an active area of research for many years [1]. This central objective is foremost in nearly all modeling applications, which transcends a multitude of engineering fields because it can be applied to problems all the way from fundamental material research up to product design. While many fields can benefit from such a model, the acceptable computational time varies based on the application and intended end user. While researchers may be able to wait weeks for a solution, product designers may be willing to wait only a matter of seconds. From continuum power-law plasticity models to highly detailed crystal plasticity, full-detailed physically based models and short computation times are often mutually exclusive.
This study explores a hardening model embedded within two crystal plasticity frameworks: a homogenized viscoplastic self-consistent (VPSC) algorithm [2] and a full-field viscoplastic model based on the fast Fourier transform (VP-FFT) [3]. Both frameworks utilize the same core set of viscoplastic crystal plasticity descriptions, relating local stress tensors to local shear rate tensors, and microstructure texture information to predict the constitutive response and texture development of the material microstructure. However, these two frameworks differ in the level of detail utilized and computation time required for simulation. The VPSC code is a serial code that can be run in seconds on a personal laptop where the effect of each grain’s environment is homogenized, while the VP-FFT microstructure is discretized to generate full-field solutions and is a parallelized code that was formulated for use on a supercomputer requiring minutes to hours to compute similar microstructures.
Constitutive laws that relate local stress tensor and crystal geometry to the local strain rate tensor control the stress-strain responses of these methods. A hardening law, contained within the constitutive law, prescribes the local stress at which shear will occur on a given slip system and evolves with accumulated strain. In order to predict the stress response of a material, the appropriate parameters for the hardening model must be developed because no theory exists to predict them a priori [4]. These parameters can be determined through manual iterative educated guessing or purely mathematical optimization. Even for a simple material response, this can be excessively time consuming. Such a method coupled with the VP-FFT code could require weeks of trial and error.
Adjusting parameters in equations, a.k.a. curve fitting, is a ubiquitous approach for development of constitutive laws in all materials, ranging from polymers [5–7] to metals [8–15] to nanocomposites [16] to geological materials [17] and even to construction materials [18]. It is used with simple [13] to complex, multiphase models [8] under loading conditions such as uniaxial tension [10], creep, and fatigue [19]. Decreasing simulation computation time during curve fitting is advantageous for quicker constitutive law development. Previous studies typically achieved this by first fitting physical parameters to analytical curves and using single element finite element (FEM) simulations [12], while others have used multi-step optimization approaches [8]. The novelty of the approach used here is a separate simulation tool in which only grain averages are computed (i.e., VPSC) compared to the full-field VP-FFT to reduce curve-fitting time. It is shown that VPSC provides an adequate first guess for the constitutive law used in the full-field VP-FFT with minimal adjustments required. We offer this work in the spirit of the Materials Genome Initiative, namely, as a method for encoding data on the mechanical behavior of materials in a form that can be used for a broad range of scientific and engineering purposes.
The remainder of this manuscript is laid out as follows. The “Background” section consists of the background and theory of the computational models utilized. The “Methods” section contains the optimization scheme in MATLAB utilized to find best-fit parameters within VPSC and a discussion of the materials investigated within this study. In the “Results and discussion” section, the results of the optimizations and how the parameters fare in the VP-FFT predictions of viscoplastic response are presented and discussed for the three materials considered. A comparison of the texture evolution between VPSC and VP-FFT is also presented. Additionally, the dependence of constitutive law parameters on the VP-FFT domain size is discussed. Finally, conclusions are provided in the “Conclusions” section.
VPSC
The VPSC computer code used in this study was developed at Los Alamos National Laboratory with applications to a range of materials such as copper, titanium, and steels [20–22] and complex loading histories [23].
Local constitutive behavior
\( {\overset{.}{\gamma}}_o \) is a normalization factor, typically assigned a value of 1, and n is the rate sensitivity exponent, typically assigned a value of 10. This constitutive equation provides a mesoscale description of the viscoplastic deformation response of a polycrystalline material aggregate.
The VPSC algorithm makes use of the Eshelby [25, 26] solution approach by treating each “grain” (i.e., crystal orientation) as an ellipsoidal inclusion contained within a homogenous medium. The homogenous medium in this case is the average response of the grains. The input list of grains (texture information) is a weighted list of orientations (parameterized as the Euler angles), and therefore, no spatial information is required or used [2]. Self-consistency is enforced through ensuring that the average strain rate of the sum of the grains is consistent with the macroscopically applied strain rate. Thus, in the VPSC model, the stresses are calculated across an average based on the collection of grains and can be fully anisotropic. It allows for each individual grain to have a local strain rate that differs from the ensemble average value, thereby weakening the boundary conditions of the Taylor model, which enforces uniform strain rate over all grains. The extent of the local variations depends on the interaction model adopted, which in this case was the affine model.
Hardening model
VP-FFT
The viscoplastic FFT method is built upon the same theorems, principles, and constitutive law as VPSC. While VPSC utilizes a homogenization (i.e., Eshelby) scheme to compute the grain average stress and strain values, the VP-FFT method uses high-resolution spatial and Fourier grids over which an FFT is performed to compute the full-field solution. Therefore, spatial resolution of the microstructure is achieved. The discretized spatial grid in VP-FFT resolves each grain at whatever resolution is deemed necessary, providing orders of magnitude more degrees of freedom and spatially resolved grain-level detail. Microstructural input for the VP-FFT is a crystal orientation for each discretized point within the domain, including a phase identifier. Phase identification is used to assign slip modes and the associated hardening parameters specific to the phase.
The VP-FFT is akin to FEM-based crystal plasticity methods, but as mentioned in the preceding paragraph, the grain structure of a material in a VP-FFT simulation is represented by a regularly discretized grid (i.e., cuboidal “elements”) while in FEM simulations arbitrarily shaped hexahedral elements are admissible. Full-field solutions satisfying local equilibrium and compatibility constrains are achieved in the VP-FFT by use of a Green’s method approach. Use of an FFT to compute the convolution integral required for the Green’s method reduces computation time and improves computational efficiency over most FEM simulations. This reduced computation time and improved efficiency, providing an efficient means for studying microstructures that require high-resolution representation, such as pearlite. Full details of the mathematics of the VP-FFT method can be found in Lebensohn [3].
With the addition of microstructural detail comes an additional computation cost. Similar methods for computing the viscoplastic response of material microstructures exist in the FEM framework; however, the primary advantage of this spectral method is efficiency and reduced computation time, especially FEM simulations of comparable sizes. The FFT method has been parallelized with the FFTW library providing additional reductions in computation times [31, 32]. These reduced computation times, regardless of the number of processors used, will not overtake the speed provided by the homogenization approach in VPSC.
Methods
Optimization method
While the extended Voce equation only requires four parameters to be optimized, the least-squares curve-fit algorithm does not guarantee a unique solution. In fact, the initial guess can influence the final solution if the function contains local minima. Thus, one must check the optimized solution to ensure that it provides a reasonable description of the stress-strain behavior, as well as satisfying the least-squares algorithm. For example, the error returned by the fitting procedure may be small, but the shape of the fitted function might suggest that extrapolation beyond the fitted range would lead to large errors.
Materials investigated
The optimization of the Voce parameters using the VPSC code and the subsequent application to the VP-FFT code is tested with three material systems: 99.9999 % pure copper, interstitial-free (IF) steel, and pearlite. Copper is selected as a fitting exercise as a proof-of-concept of the optimization scheme presented here. The τ _{0}, along with the average Taylor factor, obtained for the IF steel will be used to scale the τ _{0} value for pearlitic ferrite due to the lamellar spacing.
Copper
In a previous study [33], a well-annealed 99.9999 % pure copper specimen was prepared with a gauge section for a high-energy X-ray diffraction microscopy (HEDM) measurement under progressive tensile loading to evaluate the microstructural changes due to plastic deformation [34]. A roughly 300 × 300 × 100 voxelized domain of orientation information was measured and subsequently processed to provide phase and grain identifications for use in the VP-FFT simulation containing about 7000 grains. A weak crystallographic texture was present in the initial measurement. Therefore, deviations from sampling the orientations are considered small. A 64 × 64 × 64 extraction from the strictly solid measured domain containing 213 grains is used in this study. VPSC simulation input is a sampled list of 500 crystal orientations from the original volume, weighted evenly. The resulting stress-strain curve data generated during the previous study, out to 20 % strain, is used as the target for this material. Both computational approaches used 200 time steps with a 0.1 % strain step size.
IF steel
IF steel contains low amounts of carbon and other alloying elements, resulting in a relatively simple polycrystalline microstructure. A synthetic voxelized microstructure for use in VP-FFT was generated using DREAM3D [35] with a log-normal grain size distribution and random orientation distribution in accord with the cubic crystal symmetry. The microstructure contained 465 grains and was on a 256 × 256 × 256 voxelized domain. The resulting list of the 465 crystal orientations was used as input to VPSC. As part of the synthetic structure generation, a crystal orientation was assigned to each grain. The orientation list for VPSC input assumed equal weight of all grains. Thus, the VPSC and VP-FFT starting orientation distributions were equivalent save small variations due to the log-normal size distribution in the VP-FFT input microstructure. The stress-strain data used as the target for parameter development was a tensile test taken to 18.3 % strain [36]. VPSC and VP-FFT used 183 and 18 time steps with 0.1 and 1 % step sizes, respectively.
Pearlite
Pearlite is a lamellar structure of bcc α-Fe and orthorhombic cementite. Monolithic cementite is a brittle material, but in pearlite the lamellar structure stabilizes the cementite allowing it to deform plastically [37, 38]. Because of the computational methods used in this study, it is assumed that cementite deforms by slip.
Results and discussion
Copper
Best-fit VPSC and subsequent VP-FFT constitutive law parameters for FCC copper
VPSC | VP-FFT | |
---|---|---|
τ _{0} (MPa) | 35.8 | 35.8 |
τ _{1} (MPa) | 15.6 | 17.0 |
θ _{0} (MPa) | 321.6 | 321.6 |
θ _{1} (MPa) | 85.4 | 75.0 |
A VP-FFT simulation of the 64 × 64 × 64 subset of the measured copper specimen was performed using these parameters. Minor discrepancies are present between the VP-FFT and experimental stress-strain curves at strains less than 10 %. At strains larger than 10 %, the VP-FFT flow stress is larger than the experimental data. Adjustments to τ _{1} and θ _{1} can better align the VP-FFT with the other two datasets.
The largest difference, 10.9 MPa (4.2 % error), observed between the two computational results occurs at the final strain step. However, up to 10 % strain the two curves match quite well with a mean difference of 1.1 MPa. Initially, the results vary by 4.7 MPa (4.7 %) but quickly converge. Overall, the discrepancy between the two simulations is 4.0 MPa, on average. However, if the VPSC and VP-FFT simulations were carried out past 20 %, the curves would continue to diverge, increasing the mean discrepancy between curves.
Because VPSC operates on a per-grain basis, the mosaic spread in grain orientation as a result of plastic deformation, which has been observed during HEDM and electron backscattered diffraction (EBSD) [42–44], is not captured. Thus, the texture evolution of VPSC is expected to be an overestimate, while the local nature of VP-FFT has been shown previously to provide a more reasonable texture evolution, i.e., less rapid sharpening [3]. This may explain the deviations at high strains while maintaining good agreement at low strain.
IF steel
IF steel VPSC optimized and subsequent VP-FFT Voce hardening parameters
VPSC | VP-FFT | |
---|---|---|
τ _{0} (MPa) | 54.3 | 54.3 |
τ _{1} (MPa) | 42.2 | 40.0 |
θ _{0} (MPa) | 619.2 | 619.2 |
θ _{1} (MPa) | 106.8 | 103.0 |
Computational time required for various size models. VPSC is performed on a standard personal laptop 2.9-GHz Core i7 processor, and VP-FFT is performed on the DoD ERDC Supercomputer “Garnet” with 32 2.5-GHz AMD Interlagos Opteron processors per simulation
# grains | Resolution | VPSC (s) | VP-FFT (min) |
---|---|---|---|
100 | 32^{3} | 8 | 23.7 |
64^{3} | 8 | 91.7 | |
128^{3} | 8 | 636.1 | |
200 | 32^{3} | 14 | 22.0 |
64^{3} | 14 | 90.2 | |
128^{3} | 14 | 622.3 | |
400 | 32^{3} | 26 | 22.0 |
64^{3} | 26 | 90.2 | |
128^{3} | 26 | 628.2 |
Pearlite
The philosophy of the approach used for obtaining the Voce hardening parameters for pearlite is to first decompose an experimental plastic stress-strain curve of pearlite into separate curves for the response of pearlite and cementite using measurements of stress segregation upon loading. This is necessary due to the brittle nature of cementite in the absence of a lamellar structure. Optimization is performed on the single-phase curves individually with a composite VPSC simulation performed as a check of the optimization. While VP-FFT accounts for the grain structure and subsequent cementite lamellar network, VPSC can only do this in a limited fashion [45]. Therefore, corrections must be made to τ _{0} for both phases due to the lamellar structure. Corrections for ferrite are made with a size scale argument while corrections of cementite are made via a guess-and-check method within the VP-FFT.
Pearlite has a lamellar structure of ferrite and cementite with spacing on the order of a micrometer. Clearly, this is a complicated nano-composite, and the physics that describe the deformation of each constituent phase [46–49] suggests that more sophisticated models could be used, especially for cementite. Nevertheless, for the VPSC and VP-FFT methods that employ the extended Voce model (Eq. 3) to describe the stress-strain response, the approach developed in this manuscript offers an efficient approach to develop a constitutive relation for this class of material. Where more detailed data is available, such as multiple different strain paths, more complex models, e.g., latent hardening, may be justified.
Pearlitic ferrite is crystallographically similar to the IF steel studied above and deforms via the same slip systems. Cementite’s six primary slip modes are comprised of [001], [010], and [100] slip directions and (001), (010), and (100) slip planes. These are unique and should ideally be treated as such; however, the hardening parameters for these six slip systems are assumed to be identical for computational tractability. This assumption is also applied to the six <100> {110}^{1} and the 12 <111> {110} slip modes separately. If only the cube slip systems are included, then only three independent directions are possible (i.e., [001], [010], and [100]) and arbitrary deformation would not be possible, i.e., a von Mises criterion is not satisfied. Therefore, the inclusion of the <100> {110} and <111> {110} cementite slip modes is necessary to ensure five independent slip systems are available for slip for an arbitrary deformation. The authors know no experimental evidence that quantifiable amounts of slip occur on these modes [50–53]. To provide five independent slip systems while minimizing the slip activity on the <100> {011} and <111> {110} slip modes, τ _{0} for these modes is scaled by a factor β, which is the average ratio of the Burgers vector magnitude and interplanar spacing, b/d, for all slip systems [50] within the slip mode compared to that of <100> {001} (i.e., β for <100> {001} = 1.00). The b/d ratio is a measure of a system’s barrier to slip. An ideal slip system has a large interplanar spacing and a small Burgers vector. Hence, b/d will be small. Therefore, the τ _{0} for <100> {001} can be specified, and τ _{0} for the other slip modes is calculated. β values for <100> {011} and <111> {110} are 2.092 and 3.809, respectively.
The curve used for fitting pearlite parameters exhibits a similar behavior at low strains to the response of the IF steel curve. However, owing to the small strains tested for the IF steel, the large-strain Voce parameters (i.e., τ _{1} and θ _{1}) cannot be considered to be reliable for use in pearlitic ferrite. Therefore, a new comparison curve is selected for the large strains tested.
Cementite’s high strength and network of interconnected lamellae in the fully pearlitic microstructure will require a higher stress to achieve the prescribed overall deformation. Therefore, cementite is expected to be the limiting phase in pearlite. The apparent yield stress of cementite is ~1500 MPa [54] while the generally accepted yield stress of pearlitic ferrite without length effects is 70 MPa. Therefore, it is reasonable to expect yield stress values in cementite to be on the order of ten times larger than ferrite.
List of Voce constitutive law parameters (MPa) for pearlite
Original τ _{0} (MPa) | Final τ _{0} (MPa) | τ _{1} (MPa) | θ _{0} (MPa) | θ _{1} (MPa) | |
---|---|---|---|---|---|
Ferrite <111> {110} | 444.3 | 185.8 | 170.6 | 2027.9 | 11.0 |
Ferrite <111> {112} | 444.3 | 185.8 | 170.6 | 2027.9 | 11.0 |
Cementite <100> {001} | 322.2 | 2726.0 | 1.215 | 0.276 | 628.9 |
Cementite <100> {011} | 674.1 | 5702.1 | 1.215 | 0.276 | 628.9 |
Cementite <111> {110} | 1227.4 | 10383 | 1.215 | 0.276 | 628.9 |
While VPSC is an efficient tool for finding Voce hardening parameters, it cannot account for the load transfer that takes place in the lamellar cementite structure; thus, overestimating τ _{0} for ferrite by a factor of 2 and underestimating it for cementite by a factor of 10 for the final parameters are discussed below and listed in Table 4. This is the same factor by which the yield stress varies between pearlitic ferrite and cementite. That is to say that this is evidence that VPSC (and thus the optimization) fails to account for the structural network found in real pearlite microstructures. Therefore, these values must be adjusted within the VP-FFT or set by theory. Changes to τ _{0} of either phase do not change the hardening behavior except to translate the curve up or down in stress.
The computed τ _{0} for ferrite, 185.8 MPa, with a 0.16-μm interlamellar spacing is used in the VP-FFT simulation.
Note that, although the compositions of IF steel and pearlitic ferrite are similar, their hardening mechanisms may differ (i.e., precipitation hardening versus solid solution strengthening). Nano-indentation is a possible alternative method for estimating τ _{0} for pearlitic ferrite. However, the IF steel test data available in the literature was convenient for the estimates required for the method developed in this manuscript. Additionally, this inaccuracy in this portion of the pearlite model is likely minimal considering the much larger τ _{0} for cementite.
Due to the inability of VPSC to take into account the lamellar structure of pearlite, adjustments to cementite τ _{0} were performed via trial-and-error VP-FFT simulations. τ _{0} for the cementite <010> {001} slip mode was found through VP-FFT adjustments with an initial guess coming from VPSC. Initial CRSS values for the other slip modes are determined by the β parameter described previously. Despite the polycrystalline cementite and ferrite structures used in VPSC optimization, the remaining Voce hardening parameters, τ _{1}, θ _{0}, and θ _{1}, were constant for all slip modes of ferrite and cementite. Table 4 lists the Voce hardening parameters used for all phases and slip modes in all subsequent VP-FFT calculations. These hardening values show the control of the initial hardening rate by ferrite (i.e., small θ _{0} for cementite) and the final hardening rate by cementite (i.e., small θ _{1} for ferrite).
In comparison to Cu and IF steel, the fit to pearlite is less accurate. This may be attributed to numerous factors including the development of dislocation structures within the ferrite that control the ferrite deformation at progressively higher strains [46–49]. The VPSC and VP-FFT methods and the simple Voce hardening model (Eq. 3) do not sufficiently account for the physics of such phenomena. Additionally, there exist collinear slip directions at the ferrite-cementite interface in the Bagaryatsky orientation relationship (i.e., [010] Fe_{3}C parallel to [111] Fe) that can account for additional hardening. However, this effect of latent hardening is not accounted for in the Voce hardening model employed here. This leads to the difficulties observed in providing the excellent match between the test data and simulation responses observed in Cu and IF steel. This final case study may extend beyond the intended capabilities of the VPSC and VP-FFT methods, but the approach described in this manuscript still is useful for reducing the time required to obtain model parameters to describe the compatible deformation of a lamellar structure of ferrite and cementite.
Domain size dependence
While higher resolutions afford more degrees of freedom and higher potential for mosaic spread of crystal orientations, the viscoplastic constitutive response of the crystal is largely independent of domain resolution. For example, in the previous section the large difference in VPSC and VP-FFT model resolutions results in a very small difference in stress-strain response with equivalent Voce parameters. This is confirmed as no domain response varied by more than 2.0 MPa on average, with a maximum deviation of 3.88 MPa at 6 % strain at the lowest domain resolution. It is clear from this analysis that no dependence on domain size is present for simply polycrystalline microstructures within VP-FFT.
Note that while this work has focused on fitting the predicted stress-strain behavior, both codes also simulate texture evolution. Thus, one could utilize an optimization that tracks both stress-strain and texture, which would require two limit states as opposed to one. This would require a different optimization algorithm, but there are no obvious obstacles to implementation.
Conclusions
There is a significant difference in computational time required between the VPSC and VP-FFT codes, Table 3. Thus, this study provides a method for reducing the amount of time required to fit experimental stress-strain data with the VP-FFT code. Applying the Voce parameters optimized through the VPSC to the VP-FFT code saves the user time and removes guesswork from the fitting process.
The utilization has been illustrated through a viscoplastic self-consistent model [2] for rapid fitting of the Voce model to experimental stress-strain data through use of MATLAB’s built-in optimization toolbox. The optimized parameters were shown to be valid in the computationally time-consuming but higher fidelity VP-FFT code. For high-purity copper, the parameter values derived with VPSC were immediately usable in the VP-FFT code and only the initial CRSS value required adjustment.
Applying this method to a pearlitic, biphasic steel resulted in a drastic decrease in the amount of time required to develop an acceptable hardening model for the VP-FFT code by decreasing the number of high-resolution simulations required. The parameters derived from VPSC provided a well-informed initial guess that required minimal change in order to properly fit the experimental stress-strain curve. This demonstrated that the method is not limited to a single-phase material. With sufficient knowledge of each individual phase, a two-phase material constitutive law can be developed.
The notation for families of crystallographic planes and directions is extended here to include the set of slip planes and directions with permutations of the indices that are distinguishable within the orthorhombic cementite crystal.
Declarations
Acknowledgements
Use of the Garnet machine at the ERDC DSRC for completion of this work is gratefully acknowledged. The support of the High Performance Computing Modernization Office via the Productivity Enhancement, Technology Transfer and Training (PETTT) program is also acknowledged.
Funding
This research was supported in part (BSA) by an appointment to the Postgraduate Research Participation Program at the U.S. Army Research Laboratory administered by the Oak Ridge Institute for Science and Education through an interagency agreement between the U.S. Department of Energy and USARL. ADR acknowledges support from the National Science Foundation under DMR 1435544.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
Authors’ Affiliations
References
- Chaboche JL (2008) Int J Plast 24:1642–1693View ArticleGoogle Scholar
- Lebensohn RA, Tome CN (1993) Acta Metall 41:2611–2624View ArticleGoogle Scholar
- Lebensohn RA (2001) Acta Mater 49:2723–2737View ArticleGoogle Scholar
- Rollett AD, Rohrer GS, Suter RM (2015) MRS Bull 40(11):951–960View ArticleGoogle Scholar
- Abdul-Hameed H, Messager T, Zairi F and Nait-Abdelaziz M (2014). In: Rodrigues H, Herskovits J, Soares C.M, Guedes J.M, Araujo A, Folgado J, Moleiro F, and Madeira J.A (ed) Engineering Optimization 2014. Taylor & Francis Ltd., London, UK
- Zhang C, Moore JD (1997) Polym Eng Sci 32(2):414–420View ArticleGoogle Scholar
- Shi S, Yu D, Gao L, Chen G, Chen J, Chen X (2012) J Power Sources 213:40–46View ArticleGoogle Scholar
- Ran JO, Fu MW (2014) Int J Plast 61:1–16View ArticleGoogle Scholar
- Wang H, Wu PD, Gharghouri MA (2010) Mater Sci Eng, A 527:3588–3594View ArticleGoogle Scholar
- Wang H, Wu PD, Tome CN, Wang J (2012) Mater Sci Eng, A 555:93–98View ArticleGoogle Scholar
- Staroselsky A, Anand L (2003) Int J Plast 19:1843–1864View ArticleGoogle Scholar
- Balasubramanian S, Anand L (2012) J Mech Phys Solids 50:101–126View ArticleGoogle Scholar
- Smith A, Chen Z, Lee JY, Lee MG, Wagoner RH (2014) Int J Plast 58:100–119View ArticleGoogle Scholar
- Zhang K, Holmedal B, Hopperstad OS, Dumoulin S, Gawed J, Van Bael A, Van Houtte P (2015) Int J Plast 66:3–30View ArticleGoogle Scholar
- Gonzalez D, Simonovski J, Withers PI, Quinta Da Fonseca I (2014) Int J Plast 61:49–63View ArticleGoogle Scholar
- Yang BJ, Shin H, Kim H, Lee HK (2014) Appl Phys Lett 104:1–4Google Scholar
- Ma LJ, Liu XY, Fang Q, Xu HF, Xia HM, Li EB, Yang SG, Li WP (2013) Rock Mech Rock Eng 46:53–66View ArticleGoogle Scholar
- Sun L, Zhu Y (2013) Construct Build Mater 40:584–595View ArticleGoogle Scholar
- Barnett RA, O’Donoghue PE, Leen SB (2013) Int J Fatigue 48:192–204View ArticleGoogle Scholar
- Follansbee PS, Kocks UF (1988) Acta Metall 36:81–93View ArticleGoogle Scholar
- Lebensohn RA, Tome CN (1997) Acta Metall 45:3687–3694Google Scholar
- Lebensohn RA, Tome CN (1994) Mater Sci Eng, A 175:71–82View ArticleGoogle Scholar
- Hu L, Banovic S, Foecke T, Iadicola M and Rollett AD (2009) Proc. IDDRG 2009 International Conference, The International Deep Drawing Research Group, pp. 285-294; http://www.iddrg.com, accessed June 2016.
- Lebensohn RA, Casteñeda PP, Brenner R and Castelnau O (2011) Computational Methods for Microstructure-Property Relationships. Ghosh, Somnath, Dimiduk, Dennis, Springer US
- Eshelby JD (1957) Proc R Soc Lond A Math Phys Sci 241:376–396View ArticleGoogle Scholar
- Eshelby JD (1959) Proc R Soc Lond A Math Phys Sci 252:561–569View ArticleGoogle Scholar
- Tome CN and Lebensohn RA (2012) Manual for Code Visco-Plastic Self-Consistent (VPSC). public.lanl.gov/lebenso/VPSC7c_manual.pdf
- Voce E (1955) Metallurgia: Brit J Metals 51(307):219–226Google Scholar
- Taylor GI (1938) J Inst Met 62:307–324Google Scholar
- Rollett AD, Smith PR, James MR (1998) Mat Sci Eng A - Structural Materials Properties Microstructure and Processing 257:77–86View ArticleGoogle Scholar
- Frigo M, Johnson SG (2005) Proc IEEE 93:216–231View ArticleGoogle Scholar
- Anglin BS, Rollett AD, Lebensohn RA (2014) Comput Mater Sci 87:209–217View ArticleGoogle Scholar
- Li SF, Lind J, Hefferan CM, Pokharel R, Lienert U, Rollett AD, Suter RM (2012) J App Crys 45:1098–1108View ArticleGoogle Scholar
- Pokharel R, Lind J, Li SF, Kenesei P, Lebensohn RA, Suter RM, Rollett AD (2015) Int J Plast 67:217–234View ArticleGoogle Scholar
- Groeber MA, Jackson MA (2014) Integrating Materials and Manufacturing Innovation 3(5):1–17Google Scholar
- Morooka S, Tomota Y, Kamiyama T (2008) ISIJ Intl 48:525–530View ArticleGoogle Scholar
- Inoue A, Ogura T, Masumoto T (1973) J Jpn Inst Metals 37(8):875–882Google Scholar
- Ohashi T, Roslan L, Takahashi K, Shimokawa T, Tanaka M, Higashida K (2013) Mater Sci Eng, A 588:214–220.Google Scholar
- Bagaryatsky YA, Dokl, Akad and Nauk (1950) SSSR vol. 73: pp. 1161–1164.
- Sevillano JG, van Houtte P, Aernoudt E (1981) Prog Mater Sci 25:69–412View ArticleGoogle Scholar
- Sevillano JG (1974) PhD Thesis. Katholieke Universiteit, Leuven, Belgium, 1974
- Jin HJ, Kurmanaeva L, Schmauch J, Rösner H, Ivanisenko Y, Weissmüller J (2009) Acta Mater 57(9):2665–2672View ArticleGoogle Scholar
- Hayashi Y, Hirose Y, Setoyama D (2014) Mater Sci Forum 777:118–123View ArticleGoogle Scholar
- Pokharel R, Lind J, Kanjarla AK, Lebensohn RA, Li SF, Kenesei P, Suter RM, Rollett AD (2014) Rev Condens Matter Phys 5 5:317–346View ArticleGoogle Scholar
- Lebensohn RA, Canova GR (1997) Acta Mater 45(9):3687–3694View ArticleGoogle Scholar
- Embury JD, Fisher RM (1966) Acta Metall 14:147–159View ArticleGoogle Scholar
- Langford G (1970) Metall Trans A 1:465–477View ArticleGoogle Scholar
- Langford G (1977) Metall Trans A 8A:861–875View ArticleGoogle Scholar
- Inoue A, Ogura T, Masumoto T (1977) Metall Trans A 8A:1689–1695View ArticleGoogle Scholar
- Sevillano JG (1975) Mater Sci Eng 21:221–225View ArticleGoogle Scholar
- Mauer K, Warrington DH (1967) Philos Mag 15(134):321–327View ArticleGoogle Scholar
- Inoue A, Ogura T, Masumoto T (1976) Trans JIM 17:663–672Google Scholar
- Castelnau O, Blackman DK, Lebensohn RA and Castañeda PP (2008) J Geophys Res: Sol Earth vol. 113.
- Tomota Y, Lukáš P, Neov D, Harjo S, Abe YR (2003) Acta Mater 31:805–817View ArticleGoogle Scholar
- Elwazri AM, Wanjara P, Yue S (2005) Mater Sci Eng, A 404:91–98View ArticleGoogle Scholar
- Marder AR, Bramfitt BL (1976) Met Trans A 7A:365–372View ArticleGoogle Scholar
- Pokharel R (2013) PhD. Thesis. Carnegie Mellon University, Pittsburgh, PA, USA